Facile in-situ reduction: Crystal growth and magnetic studies of reduced vanadium (III/IV) silicates CaxLn1−xVSiO5 (Ln = Ce‒Nd, Sm‒Lu, Y)
Abeysinghe, Dileka; Smith, Mark D.; Morrison, Gregory; Yeon, Jeongho; zur Loye, Hans-Conrad; Journal of Solid State Chemistry 260 (2018) 80–86; doi:10.1016/j.jssc.2018.01.004

data_1561156
_publ_section_title
;
 Facile in-situ reduction: Crystal growth and magnetic studies of reduced
 vanadium (III/IV) silicates CaxLn1&#x2212;xVSiO5 (Ln = Ce--Nd, Sm--Lu, Y)
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              80
_journal_page_last               86
_journal_paper_doi               10.1016/j.jssc.2018.01.004
_journal_volume                  260
_journal_year                    2018
_chemical_formula_moiety         'Ca0.74 O5 Si Sm0.26 V'
_chemical_formula_sum            'Ca0.74 O5 Si Sm0.26 V'
_chemical_formula_weight         227.45
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   .
_cell_angle_alpha                90
_cell_angle_beta                 112.869(9)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.5572(19)
_cell_length_b                   8.776(3)
_cell_length_c                   6.9362(19)
_cell_measurement_reflns_used    4500
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      40.166
_cell_measurement_theta_min      4.095
_cell_volume                     367.78(19)
_computing_cell_refinement       'SAINT Version 8.34a (Bruker, 2014)'
_computing_data_collection       'Bruker APEXII v2014.9-0 (Bruker, 2014)'
_computing_data_reduction        'SAINT Version 8.34a (Bruker, 2014)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS (Sheldrick, 2008)'
_diffrn_ambient_temperature      300(2)
_diffrn_detector_area_resol_mean 10.4
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0317
_diffrn_reflns_av_unetI/netI     0.0180
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            10717
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        40.245
_diffrn_reflns_theta_max         40.247
_diffrn_reflns_theta_min         4.095
_diffrn_source                   'microfocus sealed X-ray tube'
_exptl_absorpt_coefficient_mu    7.974
_exptl_absorpt_correction_T_max  0.1174
_exptl_absorpt_correction_T_min  0.0573
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2014/4 (Bruker, 2014)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.108
_exptl_crystal_description       rod
_exptl_crystal_F_000             431
_exptl_crystal_size_max          0.140
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.040
_refine_diff_density_max         1.044
_refine_diff_density_min         -0.960
_refine_diff_density_rms         0.160
_refine_ls_extinction_coef       0.0030(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.215
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     42
_refine_ls_number_reflns         1154
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.215
_refine_ls_R_factor_all          0.0392
_refine_ls_R_factor_gt           0.0280
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0277P)^2^+1.6465P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0763
_refine_ls_wR_factor_ref         0.0793
_reflns_number_gt                954
_reflns_number_total             1154
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            4.cif
_cod_data_source_block           4
_cod_original_cell_volume        367.77(18)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               1561156
_shelx_estimated_absorpt_t_min   0.401
_shelx_estimated_absorpt_t_max   0.741
_shelx_res_checksum              10289
_shelx_hkl_checksum              19388